Micro-focussed XAFS spectroscopy to study Ni-bearing
precipitates in the metal of corroded Zircaloy-2
G. Kuri· C. Degueldre · J. Bertsch · S. Abolhassani
Received: 15 May 2009 / Accepted: 12 October 2009 / Published online: 4 November 2009 © Springer-Verlag 2009
Abstract The present work concerns an investigation of the local atomic environment of Ni-containing secondary phase precipitates (SPP) present in the metal-part of Zircaloy-2 cladding tubes. An unirradiated Zircaloy-2 and two spec-imens irradiated in a commercial nuclear power plant are characterized using μ-focussed synchrotron radiation, and by x-ray absorption fine structure (XAFS) spectroscopy. The patterns of Ni K-edge XANES and EXAFS of SPP in unir-radiated and irunir-radiated cladding are found different. Consid-ering the fact that Ni-bearing SPP in the unirradiated sam-ples are mainly Zintl phase Zr2(Fe, Ni) type, a detailed EX-AFS analysis of near-neighbor Ni atoms has been made. The result of a curve fit for the first two shells shows that about 2 Ni(Fe) and 8 Zr atoms are coordinated at 2.68 and 2.77 Å, respectively, around a central Ni atom in the SPP. XANES data analysis provides total electronic density of states at the Fermi level of unirradiated Zr2(Fe, Ni). At the Ni K-edge EXAFS spectra of irradiated SPP, however, only a single scattering peak is observed demonstrating the struc-tural disorder introduced by the neutron irradiation. The co-ordination number of the Ni neighboring shells is reduced markedly due to the formation of point and extended de-fects in the damaged SPP lattice. Dissolution of Ni from the SPP is also evident from the data. The results of this study provide a further basis for the description of both crystal-lographic and electronic structures of intermetallic second-phase precipitates found in Zr-based alloys.
PACS 61.82.Bg· 61.80.Hg · 78.70.Dm
G. Kuri ()· C. Degueldre · J. Bertsch · S. Abolhassani LNM, NES, Paul Scherrer Institute, 5232 Villigen PSI, Switzerland
e-mail:firstname.lastname@example.org Fax: +41-56-3102203
Zircaloy-2 is a zirconium-based alloy traditionally used as a cladding and core structure material in nuclear power plants [1,2]. Its application is based on zirconium’s inher-ent properties in a wide range such as excellinher-ent corrosion resistance, high melting point and toughness, low cross sec-tions for thermal neutron absorption, and exceptional stabil-ity under irradiation conditions. The material contains also several alloying elements, e.g., 1.2–1.7% Sn, 0.05–0.15% Cr, 0.07–0.20% Fe, and 0.03–0.08% Ni (all in weight% with the balance in Zr) as required to improve the prop-erties of zirconium for nuclear applications. The commer-cially used Zircaloy-2 product is commonly β-quenched in one or several of the process steps during their fabri-cations . In this context, while Sn is known to remain mostly in solid solution in the zirconium matrix, the in-herent solubility for the transition metals Cr, Fe, and Ni (which also stabilize the β-phase) is very low , and these form submicron-size secondary-phase particles or precipi-tates (SPP) together with zirconium. The intermetallic SPP found in Zircaloy-2 are Zr(Fe, Cr)2 and Zr2(Fe, Ni). The Laves phase Zr(Fe, Cr)2 has a hexagonal-closed-packed (hcp) or face-centered cubic structure. The ratio of Fe to Cr depends on the alloy composition of the bulk and the final heat treatment, normal values of Fe/Cr are about 1–2. The Ni-bearing SPP are mainly Zintl phase Zr2(Fe, Ni) type hav-ing a body-centered-tetragonal (bct) lattice structure. Un-der the in-service reactor operational conditions, Zircaloy-2 cladding behavior for water-side corrosion strongly depends on the alloy microstructure and SPP distribution. There-fore, a thorough knowledge of the crystallographic struc-ture, chemical composition, and morphology of the SPP are of special interest, since they are closely related to the cor-rosion behavior, changes in mechanical and metallurgical
properties, and hydrogen uptake of Zircaloy under neutron irradiations [5,6].
A large number of studies have been published on the evolution of precipitates during oxidation of the zirconium alloys [3,7–13]. The microstructure of the alloys was pre-dominantly observed by various analytical methods, e.g., conventional optical microscopy, transmitted light opti-cal microscopy, scanning electron microscopy (SEM), and transmission electron microscopy (TEM). The types of pre-cipitates in the alloys were identified by analyzing the se-lected area diffraction (SAD) pattern in TEM and the chem-ical composition from the energy dispersive X-ray spec-troscopy (EDS). Such studies are mostly concerned with differences in the size and distribution of SPP, including the extent of lattice deformation, and the corresponding differ-ences in microstructural developments in the Zr matrix. It has been observed that oxidation of precipitates is delayed compared to the zirconium matrix . The effect of SPP on metallurgical properties and corrosion has been also re-ported . The properties of these intermetallics under ir-radiation environment in reactor up to a high burn-up have been the subject of several investigations [15–19]. However, structural aspects concerning lattice defects and their prefer-ential location in these intermetallic phases have never been investigated. Since the sizes of these SPP are very tiny, their study for determining crystallographic structures by TEM on ultrathin specimens is often quite difficult due to the matrix contribution on the EDS spectrum and on the cor-responding electron diffraction patterns. SPP volume frac-tions in Zr alloys also are very small. Therefore, a good sta-tistic can only be obtained in TEM analysis by performing many examinations which are quite time consuming. Thus, the use of synchrotron-based X-ray absorption fine struc-ture (XAFS) spectroscopy technique is of utmost interest. The ability of XAFS, both extended X-ray absorption fine structure (EXAFS) and X-ray absorption near edge structure (XANES), to yield local structural information in an atomic scale has been well documented in the literature .
Recently, imaging of SPP in Zircaloy-2 has been carried out using nano-focussed X-ray synchrotron radiation . This allowed detection of Fe and Cr rich metallic precipi-tates with a diameter of 20 nm or greater. The Ni rich phases were not detected due to both the experimental limitations and the lower Ni concentration (compared to Fe or Cr) in the alloy. From the XANES spectra recorded for selected SPP at Fe and Cr L2,3 edges, it has been possible to esti-mate the chemical state of these impurities. From this study we were also able to demonstrate the possible lattice en-vironment (cubic and hexagonal, respectively, for Fe and Cr atoms) within the intermetallics. However, only XANES data did not provide any detailed structural information from Fe- and Cr-containing SPP . In this work, a corroded and unirradiated Zircaloy-2 was selected as a first case to
study in detail the local atomic structure of Ni-bearing SPP located at the metal side of the material. For the analysis, both EXAFS and XANES techniques have been used. Apart form the site symmetry of the absorbing atom, XANES data provide additional information about the unoccupied elec-tronic states of the material and description of Fermi level. To complement the previous information and understand the SPP behavior under irradiation environment, EXAFS spec-troscopic results of local structure around Ni atoms obtained from two irradiated specimens are also presented and quali-tatively discussed.
2.1 Materials, irradiation, and TEM
The specimens investigated here are taken from a Zircaloy-2 cladding material used in a boiling water reactor,1from the unirradiated state up to a burn-up of 66.9 MWd/kgU. The material contains several alloying elements with a nominal composition of 1.34% Sn, 0.18% Fe, 0.11% Cr, and 0.05% Ni (all in weight%) with the balance in Zr. The manufac-turing details, metallurgical characteristics, and evolution of microstructural features following various stages of neutron irradiation of these specimens can be found in one of our previous publications . Three selected samples from this batch were collected for XAFS measurements, and their re-sults are presented in this work. Details of the specimens are summarized in Table1. The as-received unirradiated sample was furthermore studied using a TEM (200 kV JEOL2010) equipped with an energy dispersive spectrometer to reveal the SPP sizes and distributions.
2.2 XAFS and data analysis
X-ray absorption experiments were performed at the un-dulator beam line X05L of the Swiss Light Source (SLS), Paul Scherrer Institute, Switzerland. The storage ring oper-ates at electron beam energy of 2.4 GeV with a maximum stored current of 400 mA. The beam line provides a micro-focussed (1μm× 1μm) spot size on the sample in the en-ergy range 5 to 20 keV, and radioactive specimens are al-lowed at this facility: these were indeed extremely impor-tant in the present work for carrying out the measurements. A fixed-exit Si(111) double-crystal Bragg monochromator cooled with liquid nitrogen was used for the energy selec-tion, the estimated energy resolution being about E/E < 0.02% at the Ni K-edge. Due to the high dilution of the al-loying elements, all XAFS measurements have been made in the fluorescence mode. The incident X-ray intensities were 1http://www.kkl.ch.
Table 1 Description of the three Zircaloy-2 cladding tube (before and after irradiation in the reactor) specimens analyzed in this study Specimen identification Number of cycles Assembly burn-up (MWd/kgU) Irradiation fluence (n/cm2for E > 1.35 MeV) Unirradiated – – – Sample-IA 3 34.7 5.9× 1021 Sample-IB 6 66.9 14.2× 1021
measured by means of an ultrathin Si-diode. The specimens were held at room temperature, and the fluorescence excita-tion spectra at the Ni K-edge were collected with an energy dispersive solid-state 32-element Ge detector. The measure-ment geometry was 45° (angle of incidence), and the de-tector was placed perpendicular to the beam direction. Inte-grated Ni fluorescent signal was optimized by changing the beam spot position (with a (sub)micron precision) on the samples. Several spectra (scans) were collected from each sample to have a better ratio signal/noise. For calibrating the energy output of the monochromator, the K-edge excitation energy of 8333 eV measured from a hyperpure nickel metal-lic foil, was set equal to the maximum of the first derivative of the XANES data.
XAFS data processing and numerical analysis were per-formed using the computer program IFEFFIT.2Considering the measurements geometry, an appropriate correction has been applied to all the measured data for the self-absorption effect . The first step in the data analysis was a back-ground subtraction. This was done using a linear function in the pre-edge region and a spline fit above the absorp-tion edge. The threshold posiabsorp-tion E0 was determined from the maximum of the first derivative of an absorption curve. Background-removed EXAFS function χ (k) was extracted and normalized by the edge jump height. χ (k) was then mul-tiplied by k3to emphasize the higher k region. Thereafter, k3-weighted EXAFS was Fourier transformed (FT) into real space to obtain a radial distribution function (RDF) of the near-neighbors around the absorber atom. Transform termi-nation effects were minimized by choosing an appropriate window range bounded by minima in |χ(k)| and using a Hanning window function that smoothed the ends of the re-gion to zero.
In the next step, the extracted experimental EXAFS signals were best fitted to the well-known EXAFS equa-tion  available within the IFEFFIT algorithm. The op-timized structural parameters, namely coordination num-ber N , interatomic distance R, Debye Waller (DW) fac-tor σ2, and E
0 (a correction to E0) were derived from the fits, taking into account both the many-electron effects and the vibrations of neighboring atoms around their equi-librium positions. Quality of the fits were judged by the EX-AFS -factor as defined in the IFEFFIT code, and the ac-2http://cars9.uchicago.edu/ifeffit/feffit.html.
ceptable values are in the order of a few percent. Theoretical scattering functions (phases and amplitudes) for quantitative EXAFS fitting were generated by the FEFF code . This theoretical approach describes the photoelectron final states by an ab initio curved-wave multiple-scattering calculation using an energy-dependent exchange-correlation for self-energy within a muffin-tin potential. In our analysis, final-state potentials at Ni K-edge were calculated using atomic clusters derived from the known atomic coordinates of Zintl phase Zr2(Fe,Ni) structures as referred in [25,26].
3 Results and discussion
3.1 Second-phase particles observation by TEM
The precipitates present in the metallic matrix of unirradi-ated Zircaloy-2 are mainly Zr(Fe,Cr)2and Zr2(Fe,Ni) with Fe/Cr and Fe/Ni ratios, respectively, close to 0.9 and 1.7. These characteristics are in good agreement with those de-scribed in our previous TEM studies  for the same al-loys. A typical TEM micrograph of this specimen and cor-responding elemental EDS mapping for Ni, Fe, and Cr are shown in Fig.1. It is straightforward to distinguish between Fe/Cr and Fe/Ni intermetallics by EDS mapping. Some of the course Fe/Ni SPP are encircled in the figure. The num-ber of Fe/Cr containing precipitates can be found larger than that of Fe/Ni particles. The precipitates also exhibit a range of sizes between 50 and 250 nm in diameter. It was con-firmed from SAD pattern that these intermetallic particles are not amorphous in nature. As alluded, investigations by TEM on the evolution of microstructure, size distribution, and dissolution of SPP under irradiation have been discussed in prior research . However, TEM observations do not allow any quantitative conclusions concerning atomic struc-tures within SPP. It is worth noting in Fig.1that Ni-bearing particles are spatially separated by more than 1μm (an aver-age value). Therefore, the structural information that is gath-ered using a micro-focussed beam spot in XAFS analysis provides average result from an isolated SPP present at the (sub)surface regions of the specimens and a couple of indi-vidual SPP perhaps located along the beam path. At the Ni K-edge energy and 45° incidence angle geometry, the esti-mated x-ray probing depth in Zircaloy-2 is about 8μm.3 3http://henke.lbl.gov/optical_constants/atten2.html.
Fig. 1 Bright field TEM micrograph and EDS elemental maps of Fe, Ni, and Cr illustrating the size distribution of Ni–Fe and Fe–Cr bearing precipitates in the unirradiated Zircaloy-2 sample analyzed in this work
3.2 EXAFS and XANES on unirradiated material
The use of unirradiated Zircaloy-2 material is essential for interpretation of EXAFS results from irradiated specimens, as they provide directly comparable structural information. In this respect, a comprehensive quantitative analysis of the XAFS data measured from this pristine specimen has been made. The results are shown in Fig.2. The upper panel in the figure reports representative Ni K-edge XAFS spectrum (Fig. 2a). The edge position, taken as equal to the maxi-mum value of the differential coefficients of the spectrum near the edge, reveals an E0 value of 8332 eV, which is 1 eV smaller than that of the Ni-metal foil (XANES spec-trum shown later). For a quantitative analysis of this data, the fitting procedure was adopted using the standard methods as summarized in the experimental section. The resulting RDF is shown in Fig.2a as an inset. The FT was performed in the spectral k range of 3–11 Å−1. The spectra drawn with points and solid curves are the observed and corresponding best-fitted ones, respectively. The lower panel (Fig.2b) plots the XANES part of the data (presented in Fig.2a) as well as the spectrum derived from FEFF calculations.
The EXAFS measurement from pristine Zircaloy-2 clearly reveals an excellent crystallinity around Ni atoms. The FT data presented in Fig.2b illustrates Fourier features which are characteristics of the bct -sites environments. The RDF shows that there are three strong amplitude peaks be-tween 2 and 7 Å, where the distance R is around 2.8, 4.8, and 6.1 Å, respectively. A small structure peaking at about 3.7 Å can be also seen in the spectrum. The first strong peak at about 2.8 Å stems from the first and second neighbors (Ni and Zr atoms, respectively) of the Zr2(Fe, Ni) lattice. The magnitude intensity of the second peak near 4.8 Å is sensi-tive to the complicated environment of Ni atoms consisting of 30 neighbors (both Ni (or Fe) and Zr) in five coordination shells. The bimodal peak around 6.1 Å contain contributions from long-range order (beyond the first seven shells).
The starting model employed to analyze these data was to use the C16-type crystal structure of Zr2Ni with space-group symmetry D184h-I4/mcm(no 140). This structure is charac-terized by a Zr2Ni unit cell, which is used in our calcula-tions, contains four Zr atoms at the positions (12− x, x, 0), (1− x,12− x, 0), (12+ x, 1 − x, 0), (x,12+ x, 0) and the Ni atoms at the positions (0, 0, 14) and (12, 12,14). Here x repre-sents the atomic parameter . For the lattice and atomic
Fig. 2 (a) Normalized and background removed Ni K-edge XAFS spectrum for the unirradiated Zircaloy-2 sample measured with a μ-focussed X-ray beam. The inset shows magnitude of the associated Fourier transform of the experimental EXAFS signal. (b) Near-edge part of the experimental XAFS data shown in (a) and the simulated XANES spectrum at the Ni K-edge obtained from FEFF code. The theoretical calculation has been carried out using a bct lattice of Zr2(Fe,Ni) structural model. See
the text for further details
parameters, we have used a= b = 6.431 Å, c = 5.418 Å, and x = 0.168. These values have been calculated using the literature data  for unit cells of pseudo-binary al-loys Zr2Fe and Zr2Ni, and taking into consideration the fact that average (atomic) ratio of Fe/Ni in the SPP yields a value of 1.45± 0.15 . The crystallographic parameters for the first five shells are given in Table2. Information about the local structure in this unirradiated sample is, thereafter, ob-tained by fitting experimental data with the corresponding atomic scattering functions calculated using FEFF  for a Zr2Fe0.6Ni0.4lattice with the crystallographic parameters just mentioned. The analysis resulted a good fit to the
exper-imental data. The starting FEFF model comprises all single scattering paths within the fit range and all multiple scatter-ing paths up to 6.0 Å. Durscatter-ing the preliminary fittscatter-ing analysis, the R, σ2, and E0of contributing atom shells were floated, while all other parameters were held fixed at their theoretical values. Once approximate values of the radial distances and DW factors were determined, additional fits were carried out in which the R and σ2values were fixed and the N , S20, and E0values were allowed to vary. Further refinement of the fit was achieved by fixing the N , S02, and σ2values at the fitted values and again varying R using the previously deter-mined values as the starting values. Finally, all parameters
Table 2 Crystallographic data of coordination numbers (N ) and inter-atomic distances (R) in crystalline Zr2Ni
Absorbing atom Neighboring atom N R(Å) Note Ni Ni 2 2.67 First five Zr 8 2.75 shells Ni 4 4.54 Zr 8 4.63 Zr 8 4.71 Zr Ni 4 2.75 15 atoms Zr 1 3.03 in five Zr 2 3.09 coordination Zr 4 3.38 shells Zr 4 3.46
Table 3 Ni EXAFS fit parameters of the first two coordination shells Specimen SC CN RD (nm) σ2(Å2) Quality identification (±0.3) (±0.002) (±15%) factor (R) Un-irradiated Ni–Ni 1.5 0.268 0.0091 0.013 Zircaloy-2 Ni–Zr 7.5 0.277 0.0145
SC: scattering configuration; CN: coordination number; RD: radial dis-tance
were floated from the starting values determined from the above approach until a best fit for all parameters was ob-tained. All data in Fig.2have also been corrected for elec-tron phase shifts using the first shell-path from FEFF, and therefore the FT peaks should correspond directly with the true bond distances of the near neighbors. At this point let us mention that Ni and Fe atoms, when compared in terms of their sizes, behave as equivalent backscatterers and are in-distinguishable from the XAFS point of view. Therefore, in our present analysis, the local environment of Ni atoms has been deduced assuming only two kinds of neighbors (Ni–Ni and Ni–Zr) for the central atom residing in a bct Zr2Ni(Fe) lattice. In this way the correlation among RNi–Ni, RNi–Fe, and
E0was reduced, and hence the number of free parameters in the fit. This approximation is reasonable, since Ni and Fe are similar in their ionic radii and have very close values of electronegativity . Therefore, the electrostatic potentials induced by charge transfer between Ni and Fe atoms can be neglected, and the approximation of neutral absorber atom assumed by FEFF is valid, so that an overall R and E0 are enough for all scattering events. Thus, the contributions from Ni–Ni correlation (for example) in the FT peak (see Table3) imply the results of Ni–Ni(Fe) atoms-shell in prac-tice, Ni being the central atom.
Table3 contains the analyzed numerical results for the first two coordination shells. The refined values obtained from the curve fit give realistic DW factors, correct order
for the bonds, and appropriate coordinations for the next-neighbor shells. The total numbers of the Ni emitter for the first two shells are NNi–Ni= 1.5 ± 0.3 and NNi–Zr= 7.5± 0.3. These values are consistent with corresponding values reported by using X-ray crystallography  and XAFS studies on crystalline nickel–zirconium alloys . The measured Ni–Ni bond distance is 2.68± 0.02 Å in the first coordination shell. Describing the RNi–Zrresult, we no-tice that the eight-fold Zr neighbors provide an average bond distance of 2.77 Å, which is significantly smaller than the sum of the elemental radii of constituting atoms (Ni, 1.35 Å; Zr, 1.55 Å4,5). This can be explained by a charge transfer from the Zr to the Ni atoms in the Zr2Ni alloy. Such an ex-planation is in accordance with the Ni–Zr interaction which is indicated by the shortened bond length with respect to the pure Ni element, and a shift of 1 eV to a lower energy of the Ni-edge position (E0value) in the SPP analyzed. Fur-ther support for this conclusion can be obtained by the local density of states calculations of Zr2Ni C16 compound . A charge transfer from the Zr 4d orbitals to the unfilled Ni 3d shell leads to a decrease of the effective Zr radius. Con-cerning the DW factors, our results indicate σ2much larger for the Ni–Zr pair (145× 10−4 Å2) compared with Ni–Ni pair (91× 10−4 Å2). For comparing these values of DW factors with the existing literature, we have not come across any report of XAFS describing the Ni environment within SPP in Zircaloy-2. The available data of σ2reported in  for Ni–Ni and Ni–Zr pairs have been measured only at low temperatures (∼77 K). Let us also note that Zr atoms are rather heavy scatterers and the Ni chains are relatively free to vibrate with respect to the Zr host lattice.
Ni K-edge experimental and calculated (using FEFF) XANES spectra of an unirradiated sample are shown in Fig.2b. Because the Fermi energy of the experimental curve is not known absolutely, the first inflection points (marked by a dotted line in the plot) of the theoretical and experi-mental curves are approximately lined up and also normal-ized to each other. Features present in the XANES spec-trum are dependent on both the local atomic arrangement around the photo absorber and the electronic states of con-stituent elements in the alloy. Furthermore, the near-edge range XANES of XAFS spectra give information about the unoccupied local density of states projected at atom sites (LDOS). The FEFF calculation itself is characterized by the following technical details. Muffin-tin exchange and corre-lation Hedin–Lundqvist potentials were used. Self consis-tency calculations were refined with a radius of 4.0 Å around the central Ni. For the full multiple-scattering calculations, we have chosen a radius of 7.2 Å to obtain about 100 atoms 4http://www.webelements.com/nickel/atom_sizes.html.
in the simulated cluster. The refined experimental parame-ters obtained from the EXAFS analysis were reintroduced in FEEF for calculation of the XANES and LDOS. Since the code was unable to reproduce the experimental XANES features during the preliminary analyses, several calculation parameters of the code were varied, aiming to analyze their influence on the theoretical spectra. After some tests, the fi-nal calculation comprised the use of a full multiple scatter-ing method [31,32], appropriate correction factors related to the Fermi level estimate (using EXCHANGE and COR-RECTIONS cards in FEFF), and the Debye temperature of Zr2Ni (252 K ) in DW factor calculations. A statistical structural disorder in the atomic layers was furthermore in-corporated with the help of the SIG2 card (a value of 0.004) in FEFF. In this way it was possible to obtain a reasonable agreement between experiment and computed spectrum, in terms of both absolute magnitudes and the line-shape. Rela-tive positions and intensities for the dominant XANES fea-tures present in the Ni-bearing SPP modeled are reproduced (see Fig.2b).
Continuing the discussion on XANES results, for Zr2Ni, we find a Fermi level (EF) of−10.9 eV with our input op-tion in LDOS calculaop-tions. In Fig.3, we show the local par-tial electron densities of states (DOS) for Ni and Zr compo-nents and the total DOS for compound Zr2Ni found from the analysis. It is clear that EFlies at a valley in DOS for Zr2Ni. The broad and three-humped pattern above Fermi level is arising predominantly from the heavier Zr atom, while the sharp peak around−2.5 eV in Fig.3a is due to the lighter atom Ni. For the alloy, total electronic DOS at EFis predom-inantly due to d-electrons on the Zr and Ni sites. Also, there is a nonzero contribution from p-DOS at the Fermi level, although in the atomic state both Zr and Ni atoms have only s- and d-electrons (3d84s2 for Ni; 4d25s2 for Zr). These results are in qualitative agreement with the band model of C16 Zr2M (M = Fe, Co, Ni, Rh) compounds [34,35] and with the electronic structure calculation of Zr2Ni us-ing the tight-bindus-ing approximations . Since the elec-tron conduction mechanism of ZrO2involving intermetallic SPP is expected to be a band mechanism, the description of the electronic structure provided here is important for ex-plaining the oxide growth resulting from oxygen migration through the oxide where the rate of oxidation is known to be controlled by either ionic or electronic conductivity of the oxide layer [5,6].
3.3 XAFS on irradiated material
Dealing with neutron irradiated samples, the RDFs ex-hibit remarkable differences in many respects. Significant radiation damage effects are readily apparent in the raw data. Figure4 displays the Ni K-edge XAFS spectra mea-sured from the two irradiated samples, which is detailed
Fig. 3 (a) The total electronic density of states (DOS) for the alloy Zr2Ni derived from the analysis. The angular momentum projected
partial l-DOS for Zr (b) and Ni (c) in the compound Zr2Ni are also
Fig. 4 Ni K-edge XAFS spectra and the corresponding Fourier transforms (inset) showing the experimental data for two neutron-irradiated samples as described in Table1
in Table1. A notable feature is the absence of any strong high-frequency contribution of experimental EXAFS sig-nals from distant coordination shells; apparently, they are smeared out by a strong static disorder. In the interval 2 to 6.5 Å, RDFs (inset in Fig. 4) show only a major peak at about 3 Å and a nonzero contribution at about 4 Å with no significant signal above this value. These structures can be attributed to the first two coordination shells around Ni atoms and to multiple-scattering effects. Our prelimi-nary analysis, however, has demonstrated that the multiple-scattering contribution is negligible and that the structures in the range 2.0–4.2 Å in Fig. 4(inset) are predominantly due to the Ni–Zr pair correlation. The contribution from Ni– Ni pair is practically negligible from EXAFS perspective. Similar behavior was earlier observed in an x-ray scattering study performed on an amorphous Zr2Ni alloy, in particular for the Ni–Ni pairs which have the smallest weighting fac-tor . Comparing the unirradiated and irradiated SPP, it is evident that a transformation towards a state of greater struc-tural disorder has taken place upon irradiation, as manifested most notably by a reduction in the EXAFS amplitudes.
Although the XAFS spectra in Fig. 4of two irradiated samples look rather similar, some definite differences can be seen from their FT data (inset in Fig. 4). A system-atic attenuation experienced by the major FT-peaks is ev-ident. The amplitude reduction is strongest for the speci-men irradiated with the highest neutron fluence (sample IB). These results can be attributed to both the dissolution of SPP and the presence of strong structural disorder in intermetal-lic Ni-compounds, causing local deformations of bond dis-tances and localization of different atomic sites in the amor-phous network within the SPP. In the literature it is discussed
that amorphization occurs because the irradiated crystalline structure gets unstable due to the accumulation of radiation damage [37,38]. The irradiation-induced dissolution is due to the increase in the number of accumulated point defects (mostly vacancies) in the matrix and the increase in the sol-ubility limits of Fe and Ni under neutron irradiation . It has to be mentioned that XAFS results presented above for the irradiated SPP are only qualitative. The parameters (e.g., N , R, or σ2) of the local structure around Ni in next-neighbor shells are not reported here not only because of the poor best-fit quality parameter () but also because of the instability of quantitative results obtained from the assumed initial lattice structure of Zr2Fe0.6Ni0.4 for the FEFF cal-culation as applied for unirradiated SPP. A detail analysis of the damage state, e.g., point and extended type of defects in-cluding anti-site irregularities  in irradiated Zr2(Fe, Ni) is underway.
X-ray absorption spectroscopy is a local probe and thus appears to be a good tool to study both crystallographic and electronic structures of submicron-size intermetallic secondary-phase precipitates (SPP) found in Zircaloy-2. In this study, μ-focussed XAFS spectroscopy has been used to investigate local structure around Ni atoms of intermetallic Zr2(Fe, Ni) SPP located at the metal-side of corroded and irradiated Zircaloy-2 specimens. Characterization of SPP in the corrosion layer and/or at the metal/metal-oxide interface remains subject of future investigations after reactor ser-vice. Two selected cladding tube specimens from fuel rods
(see Table 1for details) and one unirradiated specimen of the same material are collected for XAFS measurements. Fourier transformed (FT) Ni K-edge EXAFS spectrum of the unirradiated SPP exhibits several nearest-neighbor peaks indicating a good crystallinity around Ni atoms in the al-loy. Long-range order (beyond the first- and second-shell) is readily apparent in the FT-spectrum. A detail curve fit analy-sis shows that the Ni-sites accommodate about 1.5± 0.3 Ni atoms and 7.5± 0.3 Zr atoms in the first two consecutive neighbor shells. The measured Ni–Ni and Ni–Zr bond dis-tances are 2.68± 0.02 and 2.77 ± 0.02 Å, respectively. On the contrary, the FT-spectra of irradiated SPP are dominated by a single scattering peak. Results of preliminary analyses of EXAFS data from these irradiated material clearly show no coherent scattering contributions from beyond the Ni first neighbor shell, loss of Ni from the alloy, and a reduced co-ordination number in the Ni–Zr pair with some disruption of the average bond distances. These imply presence of strong structural disorder in intermetallic Ni-bearing SPP, causing local deformations of bond distances and localization of dif-ferent atomic sites in the amorphous network within SPP. The local structure of intermetallic SPP is an important step to understand the irradiation effects including differences between damaged state and crystalline phase, and with re-spect to the corrosion behavior of the material. It is demon-strated that XAFS can be a powerful local probe towards these aspects.
Acknowledgements The authors gratefully acknowledge Hot-Labo-ratory technical-staff at PSI for preparing the radioactive specimens and μ-XAS beam-line staff for the experimental work performed at SLS. We also appreciate the useful scientific discussion with D. Gavil-let. Our sincere thanks are to swissnuclear for financial supporting this work.
1. S.R. MacEwen, J. Faber, A.P.L. Turner, Acta Metall. 31, 657 (1983)
2. P. Hofmann, J. Nucl. Mater. 270, 194 (1999)
3. A.R. Massih, M. Dahlbäck, M. Limbäck, T. Andersson, B. Lehti-nen, Corros. Sci. 48, 1154 (2006)
4. D. Charquet, R. Hahn, E. Ortlieb, J.P. Gros, J.F. Wadier, Zirco-nium in the nuclear industry, ASTM STP, vol. 1023 (1988), p. 405 5. B. Cox, J. Nucl. Mater. 336, 331 (2005)
6. A. Yilmazbayhan, A.T. Motta, R.J. Comstock, G.P. Sabol, B. Lai, Z. Cai, J. Nucl. Mater. 324, 6 (2004)
7. D. Pecheur, F. Lefebvre, A.T. Motta, C. Lemaignan, D. Charquet, in: Zirconium in the Nuclear Industry, Tenth International
Sym-posium, ASTM STP, vol. 1245, ed. by A.M. Garde, E.D. Bradley
(1994), p. 687
8. J.H. Baek, Y.H. Jeong, J. Nucl. Mater. 304, 107 (2002)
9. M.Y. Yao, B.X. Zhou, Q. Li, W.Q. Liu, Y.L. Chu, J. Nucl. Mater. 350, 195 (2006)
10. S.A. Nikulin, V.I. Goncharov, V.A. Markelov, V.N. Shishov, Zir-conium in the Nuclear Industry, Eleventh Symposium, ASTM STP, vol. 1295 (1996), p. 695
11. H.-G. Kim, J.-Y. Park, Y.-H. Jeong, J. Nucl. Mater. 345, 1 (2005) 12. J.-Y. Park, S. Jo Yoo, B.-K. Choi, Y.H. Jeong, J. Nucl. Mater. 373,
13. R. Benaboud, P. Bouvier, J.-P. Petit, Y. Wouters, A. Galerie, J. Nucl. Mater. 360, 151 (2007)
14. Y. Hatano, M. Sugisaki, K. Kitano, M. Hayashi, Zirconium in the Nuclear Industry, Twelfth International Symposium, ASTM STP, vol. 1354 (2000), p. 901; and references therein
15. A.T. Motta, J. Nucl. Mater. 244, 227 (1997)
16. S. Shimada, Y. Etoh, K. Tomida, J. Nucl. Mater. 248, 275 (1997) 17. P. Vizcaino, A.D. Banchik, J.P. Abriata, Mater. Lett. 62, 491
(2008); and references therein
18. C. Rodriguez, D.A. Barbiric, M.E. Pepe, J.A. Kovacs, J.A. Alonso, R.H. de Tendler, Intermetallics 10, 205 (2002); and references therein
19. P. Vizcaino, A.D. Banchik, J.P. Abriata, J. Nucl. Mater. 336, 54 (2005)
20. P.A. Lee, P.H. Citrin, P. Eisenberger, B.M. Kincaid, Rev. Mod. Phys. 53, 769 (1981)
21. C. Degueldre, J. Raabe, G. Kuri, S. Abolhassani, Talanta 75, 402 (2008)
22. S. Abolhassani, D. Gavillet, F. Groeschel, P. Jourdain, H.U. Zwicky, in: International Topic Meeting on LWR Fuel Perfor-mance, Park City, UT, April 10–13 (2000), p. 470
23. C.H. Booth, F. Bridges, Phys. Scr. T 115, 202 (2005)
24. J.J. Rehr, J.M.d. Leon, S.I. Zabinsky, R.C. Albers, J. Am. Chem. Soc. 113, 5135 (1991); we have used the version 8.20
25. M.E. Kirkpatrick, D.M. Bailey, J.F. Smith, Acta Cryst. 15, 252 (1962)
26. E.E. Havinga, H. Damsma, P. Hokkelling, J. Less-Common Met. 27, 169 (1972)
27. National Institute of Standards and Technology; NIST/FIZ FindIt-code for Inorganic Crystal Structure Database (ICSD); We have used ICSD # 103712 and ICSD # 105479 for Zr2Fe and Zr2Ni,
28. J.A. Alonso, L.A. Girifalco, Phys. Rev. B 19, 3889 (1979) 29. R. Frahm, R. Haensel, P. Rabe, J. Phys. F: Met. Phys. 14, 1029
30. R. Visnov, F. Ducastelle, G. Treglia, J. Phys. F: Met. Phys. 12, 441 (1982)
31. A.L. Ankudinov, B. Ravel, J.J. Rehr, S.D. Conradson, Phys. Rev. B 58, 7565 (1998)
32. A.L. Ankudinov, J.J. Rehr, Phys. Rev. B 62, 2437 (2000) 33. R. Mittal, S.L. Chaplot, K.R. Rao, P. Raj, Physica B 222, 233
(1996); and references therein
34. H.G. Salunke, G.P. Das, P. Raj, V.C. Sahani, S.K. Dhar, Physica C 226, 385 (1994)
35. R. Mittal, S.L. Chaplot, H.G. Salunke, G.P. Das, P. Raj, A. Sathyamoorthy, K. Shashikala, S.K. Dhar, Physica C 320, 239 (1999)
36. J.C. de Lima, D. Raoux, J.M. Tonnerre, D. Udron, K.D. Machado, T.A. Grandi, C.E.M. de Campos, T.I. Morrison, Phys. Rev. B 67, 094210 (2003)
37. A.T. Motta, C. Lemaignan, in Ordering and Disordering in Alloys, ed. by A.R. Yavari (Elsevier Applied Science, London, 1992), p. 255
38. A.T. Motta, C. Lemaignan, J. Nucl. Mater. 195, 277 (1992) 39. Y. Etoh, S. Shimada, J. Nucl. Mater. 200, 59 (1993)
40. C.S. Moura, A.T. Motta, N.Q. Lam, L. Amaral, Nucl. Instrum. Methods Phys. Res. B 175–177, 526 (2001)